# Electronic Supplementary Material (ESI) for RSC Advances.
# This journal is © The Royal Society of Chemistry 2020

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Li11RbGd4Te6O30
_database_code_depnum_ccdc_archive 'CCDC 1984029'
loop_
_audit_author_name
_audit_author_address
'Jianghe Feng'
;State Key Lab Struct Chem, Fujian Inst Res Struct Matter, Chinese Acad Sci
China
;
_audit_update_record             
;
2020-02-19 deposited with the CCDC.	2020-03-16 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2018/3
_shelx_SHELXL_version_number     2018/3
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Gd12 Li33 O90 Rb3 Te18'
_chemical_formula_weight         6109.23

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      trigonal
_space_group_IT_number           167
_space_group_name_H-M_alt        'R -3 c :H'
_space_group_name_Hall           '-R 3 2"c'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z+1/2'
'x-y, -y, -z+1/2'
'-x, -x+y, -z+1/2'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'y+2/3, x+1/3, -z+5/6'
'x-y+2/3, -y+1/3, -z+5/6'
'-x+2/3, -x+y+1/3, -z+5/6'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'y+1/3, x+2/3, -z+7/6'
'x-y+1/3, -y+2/3, -z+7/6'
'-x+1/3, -x+y+2/3, -z+7/6'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z-1/2'
'-x+y, y, z-1/2'
'x, x-y, z-1/2'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-y+2/3, -x+1/3, z-1/6'
'-x+y+2/3, y+1/3, z-1/6'
'x+2/3, x-y+1/3, z-1/6'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
'-y+1/3, -x+2/3, z+1/6'
'-x+y+1/3, y+2/3, z+1/6'
'x+1/3, x-y+2/3, z+1/6'

_cell_length_a                   9.3340(2)
_cell_length_b                   9.3340(2)
_cell_length_c                   45.4665(14)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     3430.50(18)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    5863
_cell_measurement_theta_min      4.3530
_cell_measurement_theta_max      32.7140

_exptl_crystal_description       bulk
_exptl_crystal_colour            colourless
_exptl_crystal_density_meas      none
_exptl_crystal_density_method    none
_exptl_crystal_density_diffrn    5.914
_exptl_crystal_F_000             5268
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.178
_exptl_crystal_size_mid          0.149
_exptl_crystal_size_min          0.130
_exptl_absorpt_coefficient_mu    21.209
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.42393
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_process_details   
;
CrysAlisPro 1.171.39.46c (Rigaku Oxford Diffraction, 2018)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_oxdiff_exptl_absorpt_empirical_full_min 0.636
_oxdiff_exptl_absorpt_empirical_full_max 1.701
_oxdiff_exptl_absorpt_empirical_details 
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at home/near, Atlas'
_diffrn_measurement_method       'four-circle diffractometer'
_diffrn_detector_area_resol_mean 10.3503
_diffrn_reflns_number            10785
_diffrn_reflns_av_unetI/netI     0.0291
_diffrn_reflns_av_R_equivalents  0.0633
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_l_min       -62
_diffrn_reflns_limit_l_max       54
_diffrn_reflns_theta_min         4.367
_diffrn_reflns_theta_max         29.116
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measured_fraction_theta_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_point_group_measured_fraction_full 0.996
_reflns_number_total             1032
_reflns_number_gt                994
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'CrysAlisPro 1.171.39.46c (Rigaku OD, 2018)'
_computing_cell_refinement       'CrysAlisPro 1.171.39.46c (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.39.46c (Rigaku OD, 2018)'
_computing_structure_solution    SHELXTL
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_molecular_graphics    SHELXTL
_computing_publication_material  SHELXTL
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0120P)²+18.8403P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     none
_atom_sites_solution_secondary   none
_atom_sites_solution_hydrogens   none
_refine_ls_hydrogen_treatment    none
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_extinction_coef       0.000681(18)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         1032
_refine_ls_number_parameters     82
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0200
_refine_ls_R_factor_gt           0.0190
_refine_ls_wR_factor_ref         0.0456
_refine_ls_wR_factor_gt          0.0452
_refine_ls_goodness_of_fit_ref   1.200
_refine_ls_restrained_S_all      1.200
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Gd1 Gd 1.000000 1.000000 0.07707(2) 0.00529(10) Uani 1 3 d S T P . .
Gd2 Gd 1.000000 1.000000 0.15383(2) 0.00508(10) Uani 1 3 d S T P . .
Te1 Te 0.65145(3) 1.00583(3) 0.04834(2) 0.00438(10) Uani 1 1 d . . . . .
Rb1 Rb 1.000000 1.000000 0.000000 0.0119(2) Uani 1 6 d S T P . .
Li1 Li 0.666667 1.333333 0.0548(3) 0.011(2) Uani 1 3 d S T P . .
Li2 Li 0.9874(9) 1.3259(9) 0.0213(2) 0.0148(18) Uani 1 1 d . . . . .
Li3 Li 0.666667 0.6517(12) 0.083333 0.017(3) Uani 1 2 d S T P . .
O1 O 0.8863(3) 1.1287(3) 0.04814(6) 0.0079(6) Uani 1 1 d . . . . .
O2 O 0.666667 1.1476(4) 0.083333 0.0079(7) Uani 1 2 d S T P . .
O3 O 0.666667 0.8755(4) 0.083333 0.0066(7) Uani 1 2 d S T P . .
O4 O 0.6078(3) 1.1432(3) 0.02483(6) 0.0090(5) Uani 1 1 d . . . . .
O5 O 0.4176(3) 0.8736(3) 0.05385(6) 0.0073(5) Uani 1 1 d . . . . .
O6 O 0.6377(3) 0.8622(3) 0.01821(6) 0.0078(5) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Gd1 O5 2.339(3) 18_654 ?
Gd1 O5 2.339(3) 17_664 ?
Gd1 O5 2.339(3) 16_554 ?
Gd1 O1 2.361(3) . ?
Gd1 O1 2.361(3) 2_765 ?
Gd1 O1 2.361(3) 3_675 ?
Gd1 O3 2.7380(5) 2_765 ?
Gd1 O3 2.7380(5) . ?
Gd1 O3 2.7380(5) 3_675 ?
Gd2 O4 2.326(3) 36_565 ?
Gd2 O4 2.326(3) 35_545 ?
Gd2 O4 2.326(3) 34_765 ?
Gd2 O6 2.506(3) 18_654 ?
Gd2 O6 2.506(3) 16_554 ?
Gd2 O6 2.506(3) 17_664 ?
Gd2 O5 2.512(3) 18_654 ?
Gd2 O5 2.512(3) 17_664 ?
Gd2 O5 2.512(3) 16_554 ?
Te1 O4 1.864(3) . ?
Te1 O6 1.876(3) . ?
Te1 O1 1.899(3) . ?
Te1 O5 1.912(3) . ?
Te1 O2 2.029(2) . ?
Te1 O3 2.050(2) . ?
Rb1 O1 2.938(3) 21_655 ?
Rb1 O1 2.938(3) 3_675 ?
Rb1 O1 2.938(3) 19_775 ?
Rb1 O1 2.938(3) 20_565 ?
Rb1 O1 2.938(3) 2_765 ?
Rb1 O1 2.939(3) . ?
Rb1 O6 3.070(3) . ?
Rb1 O6 3.070(3) 21_655 ?
Rb1 O6 3.070(3) 3_675 ?
Rb1 O6 3.070(3) 19_775 ?
Rb1 O6 3.070(3) 20_565 ?
Rb1 O6 3.070(3) 2_765 ?
Li1 O4 2.081(10) . ?
Li1 O4 2.081(10) 2_775 ?
Li1 O4 2.081(10) 3_575 ?
Li1 O2 2.166(9) . ?
Li1 O2 2.166(9) 2_775 ?
Li1 O2 2.166(9) 3_575 ?
Li2 O1 2.008(8) . ?
Li2 O6 2.069(7) 3_675 ?
Li2 O6 2.093(9) 20_565 ?
Li2 O4 2.183(7) 2_775 ?
Li2 O5 2.319(9) 2_775 ?
Li3 O3 2.089(12) . ?
Li3 O5 2.193(3) 17_664 ?
Li3 O5 2.193(3) 3_565 ?
Li3 O1 2.302(3) 16_444 ?
Li3 O1 2.302(3) 2_765 ?


loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 Gd1 O5 77.05(11) 18_654 17_664 ?
O5 Gd1 O5 77.05(11) 18_654 16_554 ?
O5 Gd1 O5 77.04(11) 17_664 16_554 ?
O5 Gd1 O1 77.96(10) 18_654 . ?
O5 Gd1 O1 130.40(9) 17_664 . ?
O5 Gd1 O1 136.20(8) 16_554 . ?
O5 Gd1 O1 136.20(8) 18_654 2_765 ?
O5 Gd1 O1 77.96(10) 17_664 2_765 ?
O5 Gd1 O1 130.40(9) 16_554 2_765 ?
O1 Gd1 O1 91.98(10) . 2_765 ?
O5 Gd1 O1 130.40(9) 18_654 3_675 ?
O5 Gd1 O1 136.20(8) 17_664 3_675 ?
O5 Gd1 O1 77.96(10) 16_554 3_675 ?
O1 Gd1 O1 91.98(10) . 3_675 ?
O1 Gd1 O1 91.97(10) 2_765 3_675 ?
O5 Gd1 O3 129.97(7) 18_654 2_765 ?
O5 Gd1 O3 63.03(8) 17_664 2_765 ?
O5 Gd1 O3 66.05(8) 16_554 2_765 ?
O1 Gd1 O3 151.52(7) . 2_765 ?
O1 Gd1 O3 64.49(8) 2_765 2_765 ?
O1 Gd1 O3 74.08(9) 3_675 2_765 ?
O5 Gd1 O3 63.04(8) 18_654 . ?
O5 Gd1 O3 66.05(8) 17_664 . ?
O5 Gd1 O3 129.97(7) 16_554 . ?
O1 Gd1 O3 64.49(8) . . ?
O1 Gd1 O3 74.08(9) 2_765 . ?
O1 Gd1 O3 151.52(7) 3_675 . ?
O3 Gd1 O3 118.930(3) 2_765 . ?
O5 Gd1 O3 66.05(8) 18_654 3_675 ?
O5 Gd1 O3 129.97(7) 17_664 3_675 ?
O5 Gd1 O3 63.04(8) 16_554 3_675 ?
O1 Gd1 O3 74.08(9) . 3_675 ?
O1 Gd1 O3 151.52(7) 2_765 3_675 ?
O1 Gd1 O3 64.49(8) 3_675 3_675 ?
O3 Gd1 O3 118.930(3) 2_765 3_675 ?
O3 Gd1 O3 118.929(3) . 3_675 ?
O5 Gd1 Li3 92.37(14) 18_654 . ?
O5 Gd1 Li3 43.32(9) 17_664 . ?
O5 Gd1 Li3 120.01(10) 16_554 . ?
O1 Gd1 Li3 96.34(15) . . ?
O1 Gd1 Li3 45.96(12) 2_765 . ?
O1 Gd1 Li3 137.19(14) 3_675 . ?
O3 Gd1 Li3 79.07(18) 2_765 . ?
O3 Gd1 Li3 40.30(18) . . ?
O3 Gd1 Li3 157.59(16) 3_675 . ?
O5 Gd1 Li3 43.32(9) 18_654 3_675 ?
O5 Gd1 Li3 120.01(10) 17_664 3_675 ?
O5 Gd1 Li3 92.37(14) 16_554 3_675 ?
O1 Gd1 Li3 45.96(11) . 3_675 ?
O1 Gd1 Li3 137.20(14) 2_765 3_675 ?
O1 Gd1 Li3 96.34(15) 3_675 3_675 ?
O3 Gd1 Li3 157.58(16) 2_765 3_675 ?
O3 Gd1 Li3 79.07(18) . 3_675 ?
O3 Gd1 Li3 40.30(18) 3_675 3_675 ?
Li3 Gd1 Li3 119.214(2) . 3_675 ?
O5 Gd1 Li3 120.01(10) 18_654 2_765 ?
O5 Gd1 Li3 92.37(14) 17_664 2_765 ?
O5 Gd1 Li3 43.32(9) 16_554 2_765 ?
O1 Gd1 Li3 137.20(14) . 2_765 ?
O1 Gd1 Li3 96.34(15) 2_765 2_765 ?
O1 Gd1 Li3 45.97(12) 3_675 2_765 ?
O3 Gd1 Li3 40.30(18) 2_765 2_765 ?
O3 Gd1 Li3 157.59(16) . 2_765 ?
O3 Gd1 Li3 79.07(18) 3_675 2_765 ?
Li3 Gd1 Li3 119.214(3) . 2_765 ?
Li3 Gd1 Li3 119.213(5) 3_675 2_765 ?
O4 Gd2 O4 71.75(11) 36_565 35_545 ?
O4 Gd2 O4 71.75(11) 36_565 34_765 ?
O4 Gd2 O4 71.75(11) 35_545 34_765 ?
O4 Gd2 O6 76.51(9) 36_565 18_654 ?
O4 Gd2 O6 72.82(9) 35_545 18_654 ?
O4 Gd2 O6 138.11(9) 34_765 18_654 ?
O4 Gd2 O6 72.82(9) 36_565 16_554 ?
O4 Gd2 O6 138.10(9) 35_545 16_554 ?
O4 Gd2 O6 76.51(9) 34_765 16_554 ?
O6 Gd2 O6 119.060(19) 18_654 16_554 ?
O4 Gd2 O6 138.10(9) 36_565 17_664 ?
O4 Gd2 O6 76.51(9) 35_545 17_664 ?
O4 Gd2 O6 72.82(9) 34_765 17_664 ?
O6 Gd2 O6 119.058(19) 18_654 17_664 ?
O6 Gd2 O6 119.06(2) 16_554 17_664 ?
O4 Gd2 O5 95.52(9) 36_565 18_654 ?
O4 Gd2 O5 136.81(9) 35_545 18_654 ?
O4 Gd2 O5 144.58(9) 34_765 18_654 ?
O6 Gd2 O5 64.04(8) 18_654 18_654 ?
O6 Gd2 O5 68.11(8) 16_554 18_654 ?
O6 Gd2 O5 126.38(9) 17_664 18_654 ?
O4 Gd2 O5 144.58(9) 36_565 17_664 ?
O4 Gd2 O5 95.52(10) 35_545 17_664 ?
O4 Gd2 O5 136.80(9) 34_765 17_664 ?
O6 Gd2 O5 68.11(8) 18_654 17_664 ?
O6 Gd2 O5 126.38(9) 16_554 17_664 ?
O6 Gd2 O5 64.04(8) 17_664 17_664 ?
O5 Gd2 O5 70.92(10) 18_654 17_664 ?
O4 Gd2 O5 136.81(9) 36_565 16_554 ?
O4 Gd2 O5 144.57(9) 35_545 16_554 ?
O4 Gd2 O5 95.52(9) 34_765 16_554 ?
O6 Gd2 O5 126.38(9) 18_654 16_554 ?
O6 Gd2 O5 64.04(8) 16_554 16_554 ?
O6 Gd2 O5 68.11(8) 17_664 16_554 ?
O5 Gd2 O5 70.92(10) 18_654 16_554 ?
O5 Gd2 O5 70.92(10) 17_664 16_554 ?
O4 Gd2 Li1 42.58(7) 36_565 34_765 ?
O4 Gd2 Li1 42.58(7) 35_545 34_765 ?
O4 Gd2 Li1 42.58(7) 34_765 34_765 ?
O6 Gd2 Li1 95.60(6) 18_654 34_765 ?
O6 Gd2 Li1 95.60(6) 16_554 34_765 ?
O6 Gd2 Li1 95.60(6) 17_664 34_765 ?
O5 Gd2 Li1 137.95(6) 18_654 34_765 ?
O5 Gd2 Li1 137.94(6) 17_664 34_765 ?
O5 Gd2 Li1 137.94(6) 16_554 34_765 ?
O4 Gd2 Li2 103.92(17) 36_565 16_444 ?
O4 Gd2 Li2 56.28(17) 35_545 16_444 ?
O4 Gd2 Li2 125.31(16) 34_765 16_444 ?
O6 Gd2 Li2 39.86(13) 18_654 16_444 ?
O6 Gd2 Li2 156.55(14) 16_554 16_444 ?
O6 Gd2 Li2 79.35(14) 17_664 16_444 ?
O5 Gd2 Li2 89.48(15) 18_654 16_444 ?
O5 Gd2 Li2 45.56(18) 17_664 16_444 ?
O5 Gd2 Li2 116.33(17) 16_554 16_444 ?
Li1 Gd2 Li2 96.85(16) 34_765 16_444 ?
O4 Gd2 Li2 125.31(16) 36_565 18_754 ?
O4 Gd2 Li2 103.92(17) 35_545 18_754 ?
O4 Gd2 Li2 56.28(17) 34_765 18_754 ?
O6 Gd2 Li2 156.55(14) 18_654 18_754 ?
O6 Gd2 Li2 79.35(14) 16_554 18_754 ?
O6 Gd2 Li2 39.86(13) 17_664 18_754 ?
O5 Gd2 Li2 116.33(17) 18_654 18_754 ?
O5 Gd2 Li2 89.48(15) 17_664 18_754 ?
O5 Gd2 Li2 45.56(18) 16_554 18_754 ?
Li1 Gd2 Li2 96.85(16) 34_765 18_754 ?
Li2 Gd2 Li2 118.60(7) 16_444 18_754 ?
O4 Te1 O6 96.45(12) . . ?
O4 Te1 O1 99.51(12) . . ?
O6 Te1 O1 94.23(12) . . ?
O4 Te1 O5 86.98(12) . . ?
O6 Te1 O5 89.22(12) . . ?
O1 Te1 O5 172.24(13) . . ?
O4 Te1 O2 88.23(11) . . ?
O6 Te1 O2 175.24(11) . . ?
O1 Te1 O2 85.79(9) . . ?
O5 Te1 O2 90.19(9) . . ?
O4 Te1 O3 163.10(11) . . ?
O6 Te1 O3 98.23(12) . . ?
O1 Te1 O3 87.74(8) . . ?
O5 Te1 O3 84.88(8) . . ?
O2 Te1 O3 77.02(11) . . ?
O4 Te1 Li1 43.2(3) . . ?
O6 Te1 Li1 138.6(3) . . ?
O1 Te1 Li1 86.15(8) . . ?
O5 Te1 Li1 95.85(9) . . ?
O2 Te1 Li1 46.1(3) . . ?
O3 Te1 Li1 123.1(3) . . ?
O4 Te1 Li2 59.20(16) . 21_655 ?
O6 Te1 Li2 39.30(15) . 21_655 ?
O1 Te1 Li2 88.37(15) . 21_655 ?
O5 Te1 Li2 98.67(15) . 21_655 ?
O2 Te1 Li2 145.41(15) . 21_655 ?
O3 Te1 Li2 136.81(15) . 21_655 ?
Li1 Te1 Li2 99.5(3) . 21_655 ?
O4 Te1 Te1 125.90(9) . 18_654 ?
O6 Te1 Te1 137.12(8) . 18_654 ?
O1 Te1 Te1 85.86(9) . 18_654 ?
O5 Te1 Te1 86.88(9) . 18_654 ?
O2 Te1 Te1 38.12(8) . 18_654 ?
O3 Te1 Te1 38.89(8) . 18_654 ?
Li1 Te1 Te1 84.2(3) . 18_654 ?
Li2 Te1 Te1 172.91(13) 21_655 18_654 ?
O4 Te1 Li2 41.42(15) . 3_575 ?
O6 Te1 Li2 89.81(17) . 3_575 ?
O1 Te1 Li2 140.89(16) . 3_575 ?
O5 Te1 Li2 45.90(16) . 3_575 ?
O2 Te1 Li2 93.17(16) . 3_575 ?
O3 Te1 Li2 130.15(14) . 3_575 ?
Li1 Te1 Li2 66.18(18) . 3_575 ?
Li2 Te1 Li2 70.7(2) 21_655 3_575 ?
Te1 Te1 Li2 116.37(16) 18_654 3_575 ?
O4 Te1 Li3 76.85(11) . 2_665 ?
O6 Te1 Li3 128.35(19) . 2_665 ?
O1 Te1 Li3 137.39(19) . 2_665 ?
O5 Te1 Li3 39.92(19) . 2_665 ?
O2 Te1 Li3 51.92(15) . 2_665 ?
O3 Te1 Li3 87.45(7) . 2_665 ?
Li1 Te1 Li3 61.9(2) . 2_665 ?
Li2 Te1 Li3 122.26(14) 21_655 2_665 ?
Te1 Te1 Li3 64.82(5) 18_654 2_665 ?
Li2 Te1 Li3 51.58(16) 3_575 2_665 ?
O4 Te1 Li2 66.39(15) . . ?
O6 Te1 Li2 93.97(17) . . ?
O1 Te1 Li2 33.34(15) . . ?
O5 Te1 Li2 153.37(15) . . ?
O2 Te1 Li2 88.67(16) . . ?
O3 Te1 Li2 120.64(14) . . ?
Li1 Te1 Li2 64.85(17) . . ?
Li2 Te1 Li2 68.7(2) 21_655 . ?
Te1 Te1 Li2 107.93(16) 18_654 . ?
Li2 Te1 Li2 107.6(3) 3_575 . ?
Li3 Te1 Li2 126.7(2) 2_665 . ?
O1 Rb1 O1 180.00(13) 21_655 3_675 ?
O1 Rb1 O1 70.61(8) 21_655 19_775 ?
O1 Rb1 O1 109.39(9) 3_675 19_775 ?
O1 Rb1 O1 70.61(8) 21_655 20_565 ?
O1 Rb1 O1 109.39(9) 3_675 20_565 ?
O1 Rb1 O1 70.61(8) 19_775 20_565 ?
O1 Rb1 O1 109.39(9) 21_655 2_765 ?
O1 Rb1 O1 70.61(8) 3_675 2_765 ?
O1 Rb1 O1 109.39(8) 19_775 2_765 ?
O1 Rb1 O1 180.00(7) 20_565 2_765 ?
O1 Rb1 O1 109.40(8) 21_655 . ?
O1 Rb1 O1 70.60(8) 3_675 . ?
O1 Rb1 O1 180.0 19_775 . ?
O1 Rb1 O1 109.39(8) 20_565 . ?
O1 Rb1 O1 70.61(8) 2_765 . ?
O1 Rb1 O6 64.00(7) 21_655 . ?
O1 Rb1 O6 116.00(7) 3_675 . ?
O1 Rb1 O6 125.24(7) 19_775 . ?
O1 Rb1 O6 117.64(7) 20_565 . ?
O1 Rb1 O6 62.36(7) 2_765 . ?
O1 Rb1 O6 54.76(7) . . ?
O1 Rb1 O6 54.76(7) 21_655 21_655 ?
O1 Rb1 O6 125.24(7) 3_675 21_655 ?
O1 Rb1 O6 62.36(7) 19_775 21_655 ?
O1 Rb1 O6 116.00(7) 20_565 21_655 ?
O1 Rb1 O6 64.00(7) 2_765 21_655 ?
O1 Rb1 O6 117.64(7) . 21_655 ?
O6 Rb1 O6 66.99(4) . 21_655 ?
O1 Rb1 O6 125.24(7) 21_655 3_675 ?
O1 Rb1 O6 54.76(7) 3_675 3_675 ?
O1 Rb1 O6 117.64(7) 19_775 3_675 ?
O1 Rb1 O6 64.00(7) 20_565 3_675 ?
O1 Rb1 O6 116.00(7) 2_765 3_675 ?
O1 Rb1 O6 62.36(7) . 3_675 ?
O6 Rb1 O6 113.01(4) . 3_675 ?
O6 Rb1 O6 180.00(9) 21_655 3_675 ?
O1 Rb1 O6 116.00(7) 21_655 19_775 ?
O1 Rb1 O6 64.00(7) 3_675 19_775 ?
O1 Rb1 O6 54.76(7) 19_775 19_775 ?
O1 Rb1 O6 62.36(7) 20_565 19_775 ?
O1 Rb1 O6 117.64(7) 2_765 19_775 ?
O1 Rb1 O6 125.24(7) . 19_775 ?
O6 Rb1 O6 180.0 . 19_775 ?
O6 Rb1 O6 113.01(4) 21_655 19_775 ?
O6 Rb1 O6 66.99(4) 3_675 19_775 ?
O1 Rb1 O6 62.36(7) 21_655 20_565 ?
O1 Rb1 O6 117.64(7) 3_675 20_565 ?
O1 Rb1 O6 116.00(7) 19_775 20_565 ?
O1 Rb1 O6 54.76(7) 20_565 20_565 ?
O1 Rb1 O6 125.24(7) 2_765 20_565 ?
O1 Rb1 O6 64.00(7) . 20_565 ?
O6 Rb1 O6 66.99(4) . 20_565 ?
O6 Rb1 O6 113.01(4) 21_655 20_565 ?
O6 Rb1 O6 66.99(4) 3_675 20_565 ?
O6 Rb1 O6 113.01(4) 19_775 20_565 ?
O1 Rb1 O6 117.64(7) 21_655 2_765 ?
O1 Rb1 O6 62.36(7) 3_675 2_765 ?
O1 Rb1 O6 64.00(7) 19_775 2_765 ?
O1 Rb1 O6 125.24(7) 20_565 2_765 ?
O1 Rb1 O6 54.76(7) 2_765 2_765 ?
O1 Rb1 O6 116.00(7) . 2_765 ?
O6 Rb1 O6 113.01(4) . 2_765 ?
O6 Rb1 O6 66.99(4) 21_655 2_765 ?
O6 Rb1 O6 113.01(4) 3_675 2_765 ?
O6 Rb1 O6 66.99(4) 19_775 2_765 ?
O6 Rb1 O6 180.00(9) 20_565 2_765 ?
O4 Li1 O4 81.8(5) . 2_775 ?
O4 Li1 O4 81.8(5) . 3_575 ?
O4 Li1 O4 81.8(5) 2_775 3_575 ?
O4 Li1 O2 79.35(9) . . ?
O4 Li1 O2 121.48(9) 2_775 . ?
O4 Li1 O2 147.06(11) 3_575 . ?
O4 Li1 O2 147.06(11) . 2_775 ?
O4 Li1 O2 79.36(9) 2_775 2_775 ?
O4 Li1 O2 121.48(9) 3_575 2_775 ?
O2 Li1 O2 87.8(5) . 2_775 ?
O4 Li1 O2 121.48(9) . 3_575 ?
O4 Li1 O2 147.06(11) 2_775 3_575 ?
O4 Li1 O2 79.36(9) 3_575 3_575 ?
O2 Li1 O2 87.8(5) . 3_575 ?
O2 Li1 O2 87.8(5) 2_775 3_575 ?
O4 Li1 Li1 130.9(3) . 16_454 ?
O4 Li1 Li1 130.9(3) 2_775 16_454 ?
O4 Li1 Li1 130.9(3) 3_575 16_454 ?
O2 Li1 Li1 53.2(3) . 16_454 ?
O2 Li1 Li1 53.2(3) 2_775 16_454 ?
O2 Li1 Li1 53.2(3) 3_575 16_454 ?
O4 Li1 Te1 37.82(7) . . ?
O4 Li1 Te1 97.3(3) 2_775 . ?
O4 Li1 Te1 118.1(4) 3_575 . ?
O2 Li1 Te1 42.48(6) . . ?
O2 Li1 Te1 119.0(3) 2_775 . ?
O2 Li1 Te1 115.3(2) 3_575 . ?
Li1 Li1 Te1 95.6(3) 16_454 . ?
O4 Li1 Te1 118.1(4) . 2_775 ?
O4 Li1 Te1 37.82(7) 2_775 2_775 ?
O4 Li1 Te1 97.3(3) 3_575 2_775 ?
O2 Li1 Te1 115.3(2) . 2_775 ?
O2 Li1 Te1 42.49(6) 2_775 2_775 ?
O2 Li1 Te1 119.0(3) 3_575 2_775 ?
Li1 Li1 Te1 95.6(3) 16_454 2_775 ?
Te1 Li1 Te1 119.06(9) . 2_775 ?
O4 Li1 Te1 97.3(3) . 3_575 ?
O4 Li1 Te1 118.1(4) 2_775 3_575 ?
O4 Li1 Te1 37.82(7) 3_575 3_575 ?
O2 Li1 Te1 119.0(3) . 3_575 ?
O2 Li1 Te1 115.3(2) 2_775 3_575 ?
O2 Li1 Te1 42.48(6) 3_575 3_575 ?
Li1 Li1 Te1 95.6(3) 16_454 3_575 ?
Te1 Li1 Te1 119.06(9) . 3_575 ?
Te1 Li1 Te1 119.06(9) 2_775 3_575 ?
O4 Li1 Gd2 49.1(3) . 28_675 ?
O4 Li1 Gd2 49.1(3) 2_775 28_675 ?
O4 Li1 Gd2 49.1(3) 3_575 28_675 ?
O2 Li1 Gd2 126.8(3) . 28_675 ?
O2 Li1 Gd2 126.8(3) 2_775 28_675 ?
O2 Li1 Gd2 126.8(3) 3_575 28_675 ?
Li1 Li1 Gd2 180.0 16_454 28_675 ?
Te1 Li1 Gd2 84.4(3) . 28_675 ?
Te1 Li1 Gd2 84.4(3) 2_775 28_675 ?
Te1 Li1 Gd2 84.4(3) 3_575 28_675 ?
O4 Li1 Li3 96.50(9) . 3_675 ?
O4 Li1 Li3 75.54(11) 2_775 3_675 ?
O4 Li1 Li3 157.3(4) 3_575 3_675 ?
O2 Li1 Li3 52.65(14) . 3_675 ?
O2 Li1 Li3 52.65(14) 2_775 3_675 ?
O2 Li1 Li3 119.6(6) 3_575 3_675 ?
Li1 Li1 Li3 66.4(2) 16_454 3_675 ?
Te1 Li1 Li3 67.42(7) . 3_675 ?
Te1 Li1 Li3 63.32(7) 2_775 3_675 ?
Te1 Li1 Li3 161.9(5) 3_575 3_675 ?
Gd2 Li1 Li3 113.6(2) 28_675 3_675 ?
O1 Li2 O6 99.5(3) . 3_675 ?
O1 Li2 O6 101.9(3) . 20_565 ?
O6 Li2 O6 109.0(4) 3_675 20_565 ?
O1 Li2 O4 110.7(4) . 2_775 ?
O6 Li2 O4 140.9(4) 3_675 2_775 ?
O6 Li2 O4 88.9(3) 20_565 2_775 ?
O1 Li2 O5 102.5(4) . 2_775 ?
O6 Li2 O5 79.4(3) 3_675 2_775 ?
O6 Li2 O5 152.3(4) 20_565 2_775 ?
O4 Li2 O5 70.5(3) 2_775 2_775 ?
O1 Li2 Li3 53.8(2) . 3_675 ?
O6 Li2 Li3 94.9(4) 3_675 3_675 ?
O6 Li2 Li3 149.3(4) 20_565 3_675 ?
O4 Li2 Li3 84.2(3) 2_775 3_675 ?
O5 Li2 Li3 49.3(2) 2_775 3_675 ?
O1 Li2 Te1 131.6(4) . 20_565 ?
O6 Li2 Te1 84.8(3) 3_675 20_565 ?
O6 Li2 Te1 34.58(16) 20_565 20_565 ?
O4 Li2 Te1 92.7(3) 2_775 20_565 ?
O5 Li2 Te1 125.4(3) 2_775 20_565 ?
Li3 Li2 Te1 174.6(3) 3_675 20_565 ?
O1 Li2 Te1 113.7(4) . 2_775 ?
O6 Li2 Te1 110.6(3) 3_675 2_775 ?
O6 Li2 Te1 119.9(3) 20_565 2_775 ?
O4 Li2 Te1 34.40(14) 2_775 2_775 ?
O5 Li2 Te1 36.32(13) 2_775 2_775 ?
Li3 Li2 Te1 65.8(2) 3_675 2_775 ?
Te1 Li2 Te1 109.3(2) 20_565 2_775 ?
O1 Li2 Gd2 139.1(4) . 16_554 ?
O6 Li2 Gd2 50.90(18) 3_675 16_554 ?
O6 Li2 Gd2 113.6(3) 20_565 16_554 ?
O4 Li2 Gd2 90.3(2) 2_775 16_554 ?
O5 Li2 Gd2 50.66(16) 2_775 16_554 ?
Li3 Li2 Gd2 96.4(3) 3_675 16_554 ?
Te1 Li2 Gd2 79.22(19) 20_565 16_554 ?
Te1 Li2 Gd2 65.36(14) 2_775 16_554 ?
O1 Li2 Rb1 62.8(2) . . ?
O6 Li2 Rb1 66.2(2) 3_675 . ?
O6 Li2 Rb1 66.1(2) 20_565 . ?
O4 Li2 Rb1 150.4(3) 2_775 . ?
O5 Li2 Rb1 138.2(3) 2_775 . ?
Li3 Li2 Rb1 109.0(3) 3_675 . ?
Te1 Li2 Rb1 75.84(19) 20_565 . ?
Te1 Li2 Rb1 174.0(3) 2_775 . ?
Gd2 Li2 Rb1 113.6(2) 16_554 . ?
O1 Li2 Te1 31.31(14) . . ?
O6 Li2 Te1 128.9(3) 3_675 . ?
O6 Li2 Te1 81.2(2) 20_565 . ?
O4 Li2 Te1 87.1(2) 2_775 . ?
O5 Li2 Te1 114.7(3) 2_775 . ?
Li3 Li2 Te1 68.6(2) 3_675 . ?
Te1 Li2 Te1 115.7(2) 20_565 . ?
Te1 Li2 Te1 105.5(2) 2_775 . ?
Gd2 Li2 Te1 164.9(3) 16_554 . ?
Rb1 Li2 Te1 74.13(15) . . ?
O1 Li2 Li1 74.4(3) . . ?
O6 Li2 Li1 155.5(4) 3_675 . ?
O6 Li2 Li1 95.5(3) 20_565 . ?
O4 Li2 Li1 36.3(2) 2_775 . ?
O5 Li2 Li1 78.9(3) 2_775 . ?
Li3 Li2 Li1 62.1(3) 3_675 . ?
Te1 Li2 Li1 117.2(3) 20_565 . ?
Te1 Li2 Li1 54.13(12) 2_775 . ?
Gd2 Li2 Li1 119.5(2) 16_554 . ?
Rb1 Li2 Li1 126.8(2) . . ?
Te1 Li2 Li1 53.31(12) . . ?
O3 Li3 O5 81.2(3) . 17_664 ?
O3 Li3 O5 81.2(3) . 3_565 ?
O5 Li3 O5 162.4(6) 17_664 3_565 ?
O3 Li3 O1 89.2(3) . 16_444 ?
O5 Li3 O1 97.52(12) 17_664 16_444 ?
O5 Li3 O1 82.23(11) 3_565 16_444 ?
O3 Li3 O1 89.2(3) . 2_765 ?
O5 Li3 O1 82.23(11) 17_664 2_765 ?
O5 Li3 O1 97.52(12) 3_565 2_765 ?
O1 Li3 O1 178.3(6) 16_444 2_765 ?
O3 Li3 O2 144.50(16) . 2_765 ?
O5 Li3 O2 70.97(18) 17_664 2_765 ?
O5 Li3 O2 125.2(4) 3_565 2_765 ?
O1 Li3 O2 115.4(3) 16_444 2_765 ?
O1 Li3 O2 66.08(17) 2_765 2_765 ?
O3 Li3 O2 144.50(16) . 3_565 ?
O5 Li3 O2 125.1(4) 17_664 3_565 ?
O5 Li3 O2 70.97(18) 3_565 3_565 ?
O1 Li3 O2 66.07(17) 16_444 3_565 ?
O1 Li3 O2 115.4(3) 2_765 3_565 ?
O2 Li3 O2 71.0(3) 2_765 3_565 ?
O3 Li3 Li2 88.8(3) . 16_444 ?
O5 Li3 Li2 53.31(17) 17_664 16_444 ?
O5 Li3 Li2 126.25(19) 3_565 16_444 ?
O1 Li3 Li2 44.72(16) 16_444 16_444 ?
O1 Li3 Li2 135.23(17) 2_765 16_444 ?
O2 Li3 Li2 91.6(2) 2_765 16_444 ?
O2 Li3 Li2 90.2(2) 3_565 16_444 ?
O3 Li3 Li2 88.9(3) . 2_765 ?
O5 Li3 Li2 126.25(19) 17_664 2_765 ?
O5 Li3 Li2 53.31(17) 3_565 2_765 ?
O1 Li3 Li2 135.23(17) 16_444 2_765 ?
O1 Li3 Li2 44.72(16) 2_765 2_765 ?
O2 Li3 Li2 90.2(2) 2_765 2_765 ?
O2 Li3 Li2 91.6(2) 3_565 2_765 ?
Li2 Li3 Li2 177.7(5) 16_444 2_765 ?
O3 Li3 Gd1 57.97(17) . 16_444 ?
O5 Li3 Gd1 121.2(3) 17_664 16_444 ?
O5 Li3 Gd1 47.05(13) 3_565 16_444 ?
O1 Li3 Gd1 47.51(12) 16_444 16_444 ?
O1 Li3 Gd1 131.3(3) 2_765 16_444 ?
O2 Li3 Gd1 157.1(3) 2_765 16_444 ?
O2 Li3 Gd1 86.69(8) 3_565 16_444 ?
Li2 Li3 Gd1 83.24(18) 16_444 16_444 ?
Li2 Li3 Gd1 95.53(19) 2_765 16_444 ?
O3 Li3 Gd1 57.97(17) . . ?
O5 Li3 Gd1 47.05(13) 17_664 . ?
O5 Li3 Gd1 121.2(3) 3_565 . ?
O1 Li3 Gd1 131.3(3) 16_444 . ?
O1 Li3 Gd1 47.51(12) 2_765 . ?
O2 Li3 Gd1 86.69(8) 2_765 . ?
O2 Li3 Gd1 157.1(3) 3_565 . ?
Li2 Li3 Gd1 95.53(19) 16_444 . ?
Li2 Li3 Gd1 83.24(19) 2_765 . ?
Gd1 Li3 Gd1 115.9(3) 16_444 . ?
O3 Li3 Li1 156.4(2) . 1_545 ?
O5 Li3 Li1 112.7(3) 17_664 1_545 ?
O5 Li3 Li1 84.0(3) 3_565 1_545 ?
O1 Li3 Li1 106.9(4) 16_444 1_545 ?
O1 Li3 Li1 74.6(3) 2_765 1_545 ?
O2 Li3 Li1 41.8(2) 2_765 1_545 ?
O2 Li3 Li1 41.8(2) 3_565 1_545 ?
Li2 Li3 Li1 114.7(4) 16_444 1_545 ?
Li2 Li3 Li1 67.6(3) 2_765 1_545 ?
Gd1 Li3 Li1 121.45(14) 16_444 1_545 ?
Gd1 Li3 Li1 116.77(15) . 1_545 ?
Te1 O1 Li2 115.3(2) . . ?
Te1 O1 Li3 111.1(3) . 3_675 ?
Li2 O1 Li3 81.5(3) . 3_675 ?
Te1 O1 Gd1 111.53(12) . . ?
Li2 O1 Gd1 132.9(2) . . ?
Li3 O1 Gd1 86.5(2) 3_675 . ?
Te1 O1 Rb1 107.49(11) . . ?
Li2 O1 Rb1 79.7(3) . . ?
Li3 O1 Rb1 141.3(3) 3_675 . ?
Gd1 O1 Rb1 82.00(8) . . ?
Te1 O2 Te1 103.75(15) 18_654 . ?
Te1 O2 Li1 91.4(3) 18_654 16_454 ?
Te1 O2 Li1 164.6(3) . 16_454 ?
Te1 O2 Li1 164.6(3) 18_654 . ?
Te1 O2 Li1 91.4(3) . . ?
Li1 O2 Li1 73.7(6) 16_454 . ?
Te1 O2 Li3 96.86(10) 18_654 2_665 ?
Te1 O2 Li3 89.93(10) . 2_665 ?
Li1 O2 Li3 85.60(13) 16_454 2_665 ?
Li1 O2 Li3 85.60(13) . 2_665 ?
Te1 O2 Li3 89.93(10) 18_654 3_675 ?
Te1 O2 Li3 96.87(10) . 3_675 ?
Li1 O2 Li3 85.60(13) 16_454 3_675 ?
Li1 O2 Li3 85.60(14) . 3_675 ?
Li3 O2 Li3 169.0(3) 2_665 3_675 ?
Te1 O3 Te1 102.21(16) 18_654 . ?
Te1 O3 Li3 128.89(8) 18_654 . ?
Te1 O3 Li3 128.89(8) . . ?
Te1 O3 Gd1 93.93(4) 18_654 16_444 ?
Te1 O3 Gd1 96.43(4) . 16_444 ?
Li3 O3 Gd1 81.73(7) . 16_444 ?
Te1 O3 Gd1 96.43(4) 18_654 . ?
Te1 O3 Gd1 93.93(4) . . ?
Li3 O3 Gd1 81.73(7) . . ?
Gd1 O3 Gd1 163.46(15) 16_444 . ?
Te1 O4 Li1 99.0(3) . . ?
Te1 O4 Li2 104.2(2) . 3_575 ?
Li1 O4 Li2 105.3(2) . 3_575 ?
Te1 O4 Gd2 153.84(15) . 28_675 ?
Li1 O4 Gd2 88.3(3) . 28_675 ?
Li2 O4 Gd2 98.0(2) 3_575 28_675 ?
Te1 O5 Li3 106.1(3) . 2_665 ?
Te1 O5 Li2 97.8(2) . 3_575 ?
Li3 O5 Li2 77.4(2) 2_665 3_575 ?
Te1 O5 Gd1 115.33(12) . 16_444 ?
Li3 O5 Gd1 89.6(2) 2_665 16_444 ?
Li2 O5 Gd1 146.7(2) 3_575 16_444 ?
Te1 O5 Gd2 102.51(11) . 16_444 ?
Li3 O5 Gd2 147.5(3) 2_665 16_444 ?
Li2 O5 Gd2 83.8(2) 3_575 16_444 ?
Gd1 O5 Gd2 91.96(9) 16_444 16_444 ?
Te1 O6 Li2 127.9(3) . 2_765 ?
Te1 O6 Li2 106.1(2) . 21_655 ?
Li2 O6 Li2 123.0(3) 2_765 21_655 ?
Te1 O6 Gd2 103.85(11) . 16_444 ?
Li2 O6 Gd2 89.2(2) 2_765 16_444 ?
Li2 O6 Gd2 95.1(2) 21_655 16_444 ?
Te1 O6 Rb1 103.31(10) . . ?
Li2 O6 Rb1 75.7(2) 2_765 . ?
Li2 O6 Rb1 75.4(2) 21_655 . ?
Gd2 O6 Rb1 152.76(10) 16_444 . ?

_refine_diff_density_max         1.072
_refine_diff_density_min         -1.656
_refine_diff_density_rms         0.299


_exptl_crystal_recrystallization_method 'From the Melt'
_exptl_crystal_preparation       'Magnetic properties'
